Facile synthesis of efficient Co3O4 nanostructures using the milky sap of Calotropis procera for oxygen evolution reactions and supercapacitor applications

The preparation of Co3O4 nanostructures by a green method has been rapidly increasing owing to its promising aspects, such as facileness, atom economy, low cost, scale-up synthesis, environmental friendliness, and minimal use of hazardous chemicals. In this study, we report on the synthesis of Co3O4 nanostructures using the milky sap of Calotropis procera (CP) by a low-temperature aqueous chemical growth method. The milky sap of CP-mediated Co3O4 nanostructures were investigated for oxygen evolution reactions (OERs) and supercapacitor applications. The structure and shape characterizations were done by X-ray diffraction (XRD), scanning electron microscopy (SEM), energy-dispersive spectroscopy (EDS), and X-ray photoelectron spectroscopy (XPS) techniques. The prepared Co3O4 nanostructures showed a heterogeneous morphology consisting of nanoparticles and large micro clusters. A typical cubic phase and a spinel structure of Co3O4 nanostructures were also observed. The OER result was obtained at a low overpotential of 250 mV at 10 mA cm−2 and a low Tafel slope of 53 mV dec−1. In addition, the durability of 45 hours was also found at 20 mA cm−2. The newly prepared Co3O4 nanostructures using the milky sap of CP were also used to demonstrate a high specific capacitance of 700 F g−1 at a current density of 0.8 A g−1 and a power density of 30 W h kg−1. The enhanced electrochemical performance of Co3O4 nanostructures prepared using the milky sap of CP could be attributed to the surface oxygen vacancies, a relatively high amount of Co2+, the reduction in the optical band gap and the fast charge transfer rate. These surface, structural, and optical properties were induced by reducing, capping, and stabilizing agents from the milky sap of CP. The obtained results of OERs and supercapacitor applications strongly recommend the use of the milky sap of CP for the synthesis of diverse efficient nanostructured materials in a specific application, particularly in energy conversion and storage devices.


Introduction
From the Stone Age to nano era, energy is one of the most essential elements for the sustainability of life and environment. The use of energy relaxes and confronts the daily activities performed by us. Therefore, the demand for energy has increased rapidly over time due to the high population density of human beings and the development of a large number of industries. [1][2][3][4][5] Most of the energy for our activities is provided entirely using fossil fuels, and therefore, fossil fuel deposits become smaller over time, and we cannot fulll the requirement of energy from the fossil fuels. This critical scenario of increasing energy demands, depletion of fossil fuels, and their adverse impact on our environment necessitates the search for new alternative and renewable energy sources. [6][7][8] Alternative energies are very sustainable and have been available since the beginning of the universe. However, there are certain barriers for the direct capitalization of available alternative energies. These alternative energies include solar, wind, water splitting, hydro power, and nuclear. [9][10][11][12] Water splitting seems to be an emerging technology for liing other technologies such as fuel cells and metal air batteries. Water splitting is a simple, efficient, and inexpensive method to strengthen renewable energy reservoirs. [13][14][15][16][17] This proceeds via two well-known half-cell reactions, namely, hydrogen evolution reactions (HERs) and oxygen evolution reactions (OERs). [18][19][20][21][22][23][24] From a thermodynamic point of view, the HER is simple as it uses twoelectron transfer during the reaction, whereas the OER involves four-electron transfer during the reaction, [25][26][27][28] and hence, the OER is very complicated and kinetically slow. Therefore, water splitting needs an active electrocatalyst for the realization of efficient HER and OER processes. To date, the state-of-the-art electrocatalysts for the HER are Pt-based materials and for the OER are Ru/Irbased materials. [29][30][31][32][33][34] These noble metal-based materials are scarce in nature and very expensive, and thus, they cannot be used for large-scale water splitting. Many efficient nonprecious electrocatalysts are reported for the HER, but we still need efficient non-noble electrocatalysts for the OER, since it is very difficult to transfer four electrons and form a double bond during the production of O 2 molecules from water splitting. Research in this area is at its peak; however, the success for the practical production of O 2 is still far from realization. Therefore, we must increase our efforts to develop efficient nonprecious catalysts from earthabundant materials for the efficient OER. The transition metal oxides of iron, cobalt, nickel, and copper are active for the OER, but their performance is still inferior to that of the noble materials. Various electrocatalysts doped with cobalt oxide such as CoO 2 , Co (PO 3 ) 4 , CuCo 3 O 4 , NiCo 3 O 4 , and MnCo 2 O x are reported in the available literature. [35][36][37][38][39][40][41][42] These studies show that these materials are neither stable nor durable under alkaline or acidic conditions. Several methods have been used to synthesize various metal oxides including solvent evaporation, electrochemical, hydrothermal, sol-gel, co-precipitation, and green-mediated approaches. The green production of metal oxides is among the synthetic methods with several advantageous features such as inexpensiveness, environmental friendliness, and simplicity. They are used very intensively in the present time. 43 Large types of metal oxides have been synthesized by a green-mediated approach such as ZnO, Fe 2 O 3 , AgO, CuO, and Al 2 O 3 using different plant extracts of Agathosma betulina, Sida cordifolia, Pedalium murex, Gloriosa superba, and Prunus yedoensis. 44 The synthesis of different metal oxides such as ZnO, Fe 2 O 3 , AgO, CuO, and Al 2 O 3 using various plant extracts has enhanced the functional properties of these materials towards specic application. This shows a strong motivation to adopt the use of new plant leaf extracts or fruit juice to improve the electrochemical properties of nanostructured materials, because the green-mediated approach offers a wide range of useful aspects in tuning the electrochemical performance of nanostructured materials such as the plentiful availability of reducing, capping, stabilizing and structure-orienting agents from various plant parts such as stems, leaves, owers, fruits, and seeds. 45,46 These benecial phytochemicals from the plants prevent aggregation and control the shape and dimension of nanostructured materials. [45][46][47] However, there is less attention paid to the use of green-mediated approach towards the synthesis of cobalt oxide (Co 3 O 4 ) nanostructures and the role of greenmediated approach towards the enhancement in the electrochemical activity of Co 3 O 4 nanostructures. Fortunately, Co 3 O 4 is more stable and durable in alkaline media; 48-52 however, its OER activity is low, hence new strategies and methods are required to accelerate the OER kinetics on the surface of Co 3 O 4 . In addition, Co 3 O 4 is one of the transition metal oxides that have a high theoretical specic capacitance of about 3560 F g −1 . [53][54][55] The capacitance of Co 3 O 4 in the practical applications is quite low compared to its theoretical value due to its restricted electron transfer, low electrical conductivity, limited surface area, contraction and large volume expansion, and aggregation of particles. 56-60 These limitations of Co 3 O 4 enabled the sluggish kinetics, poor capacitance and cycling stability during electrochemical testing. Therefore, the capacitance of Co 3 O 4 needs to be increased by adapting new synthetic pathways. Among the abandoned plants, Calotropis procera (CP) is a species of owering plant belonging to the family Apocynaceae that is native to North Africa, Pakistan, tropical Africa, Western Asia, South Asia, and Indochina. The main phytochemical components of CP include saponin, tannin, alkaloids, oxalate, phytate and cyanogenic glycosides. Many of these phytochemicals from CP have properties like reducing, stabilizing, and chelating agents; hence, they have been successfully used to enhance the electrochemical performance of Co 3 O 4 nanostructures. The molecular structures of major phytochemicals in the milky sap of CP are drawn as shown in Scheme 1.
The use of natural products of the milky sap of CP to change the morphologies and electrochemical properties of Co 3 O 4 is not reported; hence, it was used in the current work to tune the surface and optical structure of Co 3 O 4. The ingredients of the milky sap of CP have improved Co 3 O 4 electrical conductivity, created structural defects, improved catalytic sites, enhanced cycling stability, and lowered the OER overpotential for water oxidation in alkaline media.
In this study, we used the milky sap of CP as a surfacemodifying reagent for Co 3 O 4 nanostructures during the lowtemperature aqueous chemical growth method. The ingredients of the milky sap of CP have improved the surface area, electrical conductivity, and OER activity of Co 3 O 4. The physical structure of Co 3 O 4 has been studied using different characterization techniques such as SEM, XRD, and EDS. The nanostructured Co 3 O 4 showed excellent OER activity, with a low overpotential of 250 mV at 10 mA cm −2 , and a low Tafel slope of 53 mV dec −1 . A low Tafel slope of Co 3 O 4 indicates a fast OER kinetics for practical applications. Co 3 O 4 turned out to be very stable for a period of 45 hours and showed a low charge transfer resistance. The use of natural products of the milky sap of CP could be of great importance for the synthesis of a wide range of energy storage and conversion materials.
collected from the mountains of Jamshoro, Sindh Pakistan. All the desired solutions were prepared in deionized water.

Synthesis of Co 3 O 4 nanostructures using the milky sap of CP
In a typical synthesis, an equimolar (0.1 M) solution of cobalt chloride hexahydrate and urea solutions were prepared in 100 mL of deionized water in three separate 250 mL beakers. In two beakers, 1 mL and 2 mL of milky sap of CP were placed and they were labeled as sample 1 and sample 2 respectively. However, one beaker without the milky sap of CP was named pure sample. Then, these three beakers were sealed with aluminum foil and low-temperature aqueous chemical growth method was carried out in a preheated electric oven at 90°C for  hours. Aerwards, the grown product was obtained on lter paper, washed with deionized water and dried overnight. Then, cobalt hydroxide was thermally decomposed at 500°C in air for 5 hours, and nally, a black nanostructured product of Co 3 O 4 was obtained. The synthesis process of Co 3 O 4 is shown in Scheme 2.

Physical characterization of the prepared Co 3 O 4 material using the milky sap of CP
The surface and crystal structures of the prepared Co 3 O 4 material were investigated using a variety of analytical techniques such as XRD and SEM. The XRD experiment was performed with 1.5418 Å CuKa radiations at 45 kV and 45 mA. A SEM was used at an accelerating voltage of 3 kV, and an EDS equipped with a SEM was used to identify the chemical entities. The electrochemical characterization of the prepared Co 3 O 4 materials was performed by cyclic voltammetry (CV) at 10 mV s −1 , linear sweep voltammetry (LSV) at 5 mV s −1 , and chronopotentiometry at 10 mA cm −2 , and electrochemical impedance spectroscopy (EIS) was performed at 100 kHz to 1 Hz with an amplitude of 5 mV and OER onset potential in alkaline media. X-ray photoelectron spectroscopy (XPS) was performed for quantitative and chemical state information on the surface using an ESCA 5701 unit, Physical Electronics (PHI) working with monochromatic X-ray source Al (k-alpha) of photons at 1486 eV under ultra-high vacuum at a pressure of 10-10 mbar. The obtained XPS experimental results were analyzed using 0.651 eV Au 4f 7/2 line of full width at half maximum. The UVvisible absorbance spectra were recorded using a UV-visible spectrophotometer (Lambda365, PerkinElmer, Waltham, MA, USA). The vibration bands of the Co 3 O 4 material were obtained using a Fourier transform infrared (FTIR) instrument (Tensor 27, Bruker Optics, Karlsruhe, Germany).

Electrocatalysis and capacitance analysis on Co 3 O 4 nanostructure materials
A three-electrode electrochemical cell assembly was fabricated using silver-silver chloride as the reference electrode, a platinum plate as the counter electrode, and a glassy carbon electrode (GCE) as the working electrode. The electrolyte was 1 M KOH de-aerated with N 2 . The ink of different Co 3 O 4 materials was prepared by dispersing 5 mg in 2.5 mL of deionized water and 50 mL of 5% Naon. The GCE was polished with 0.05m alumina slurry and silicon paper. Then, 5 mL catalyst ink was coated onto the GCE by a drop-casting method. The modied GCE was ready for electrochemical measurements. CV was used rst to conrm the stability of the material on the GCE, followed by LSV at slow scan to measure the OER activity. For measuring the electrochemically active surface area, CV was carried out at different scan rates. For monitoring the durability, chronopotentiometry was used at constant 10 mA cm −2 . To understand the charge transport at the interface of the modied GCE and electrolyte, EIS was performed for the frequency range from 100 kHz to 1 Hz at an amplitude of 5 mV and OER onset potential as bias. All electrochemical tests were performed in 1.0 M KOH at room temperature. The measured silver-silver chloride potential is reported in reversible hydrogen electrode (RHE) using the Nernst equation. The capacitance experiments

Physical studies of the morphology and crystalline aspects of Co 3 O 4 nanostructures prepared with the milky sap of CP
The morphological studies of different Co 3 O 4 nanostructures prepared with the milky sap of CP were performed using a SEM experimental tool, and the typical shape features recorded for pure Co 3 O 4, sample 1 and sample 2 are shown in Fig. 1a-c. It is evident that pure Co 3 O 4 has nanorods covered by dense clusters that are several microns in size, indicating a high degree of heterogeneity of the pure sample. The morphology of Co 3 O 4 made with different volumes of the milky sap of CP shows different shape orientations. The nanorods are lost and the clusters have been found for both the samples of Co 3 O 4 prepared with 1 mL and 2 mL of CP, as shown in Fig. 1b and c. It is also evident that the size of the Co 3 O 4 nanoparticles is smaller than that of the pure Co 3 O 4 sample, conrming the role of CP's reducing, capping, and stabilizing agents in controlling the shape and size of nanostructured materials. From the SEM analysis, the use of phytochemicals from the milky sap of CP is highly favorable for enhancing the catalytic performance of nanostructured materials. The phase and purity of different  shown negligible effects on the average crystallite size of sample 1 and sample 2, whereas pure Co 3 O 4 possessed a higher crystallite size value than that of sample 1 and sample 2. From this information, it is obvious that the crystallite size did not play any role in the electrochemical performance of sample 1.
Different symbols in the above-mentioned equation refer to specic variable and constant values such as A as a constant, a is the absorption coefficient, hn is the photon energy and E g, is the band gap energy and n is a constant value assigned to   2 were in the order of 2.83 eV, 2.03 eV and 2.47 eV respectively, which again indicates the role of different volumes of the milky sap of CP on the optical features of Co 3 O 4. Sample 1 was associated with a low optical band gap and would possess high conductance because Co 3 O 4 is a semiconducting material and its electrical conductance is highly dependent on the optical band gap value. The variation in the volume of milky sap during the synthesis of Co 3 O 4 has shown more pronounced surface plasmon bands, which could be associated with differences in the reduction characteristics, enhancement in the nucleation and size of crystals resulting from the oxygen vacancies, and surface defects, and hence, a difference in band gap calculation was observed. A FTIR study was conducted to evaluate the Co-O chemical binding properties of Co 3 O 4 prepared with and without the milky sap of CP, as shown in Fig. 4. The FTIR spectra of all samples were recorded in the wave number range from 400 to 4000 cm −1 . Several main vibrational bands were observed and corresponded to the presence of Co 3 O 4 in each sample. The O-H stretching band positioned at 3437 cm −1 and 1637 cm −1 was assigned to absorb water molecules, as shown in Fig. 4. The nitrogen groups were also found at the band position of 1450 cm −1 and another connected 1126 cm −1 to the Co-OH coordinated bond. Typical metal-oxygen bands were noted at 450-650 cm −1 . The FTIR study has described the presence of two bands associated with the octahedral and tetrahedral positions of Co 3+ and Co 2+ respectively, and this information has conrmed the formation of spinel structure Co 3 O 4 . 67 The FTIR analysis was fully supported by previous studies. [68][69][70] The chemical composition and oxidation states of the different elements on the surface for the as-prepared pure Co 3 O 4 and sample 1 were evaluated by XPS, and the corresponding signals are shown in Fig. 5. The wide scan survey spectra of pure Co 3 O 4 and sample 1 are similar, where the presence of Co, O and C elements are evidenced in Fig. 5a. Highresolution spectra enabled the identication of the chemical states of cobalt and oxygen on the surface. In the case of Co 2p core level signals, the spectra were decomposed into three spinorbit doublets (2p 3/2 -2p 1/2 ) along with the corresponding shakeup satellites, consistent with a cobalt spinel structure and well conrmed by previous studies, 71,72 as shown in Fig. 5b. By comparing the corresponding Co 3+ /Co 2+ atomic ratios for pure Co 3 O 4 , 1.22, and A sample, 0.80, Co 3 O 4 prepared with the milky sap of CP is richer in Co 2+ at the surface. The high-resolution O 1s spectra for pure Co 3 O 4 and sample 1 were also measured (Fig. 5c) and different types of oxygen environments such as lattice oxygen, surface oxygen, and chemisorbed oxygen were observed for both samples. 73 This signal indicates that sample 1 shows major contribution from the oxygen surface (signal at ca. 531 eV), which is normally attributed to surface defects/ vacancies. In this regard, the corresponding O Sur /O Lat atomic ratio changed from 0.6 to 1.0 for pure Co 3 O 4 and sample 1,  respectively. Therefore, the presented data indicate that the milky sap of CP has induced the formation of a surface richer on Co 2+ and oxygen vacancies, which could play an important role in the OER.

OER half-cell investigation of milky sap of CP-mediated sCo 3 O 4 nanostructures
The OER activity for pure Co 3 O 4 , sample 1 and sample 2 was measured in a three-electrode cell setup with 1.0 M KOH by LSV at 5 mV s −1 (see Fig. 6a). The measured onset potentials for sample 1, sample 2 and pure Co 3 O 4 are 1.45 V versus RHE, 1.48 V versus RHE and 1.51 V versus RHE respectively. The low OER onset potential for sample 1 suggests its excellent catalytic features, which could be attributed to the dynamic morphology, rich active sites and enhanced electrical conductivity using the Sodom apple as a surface modier. The over potentials calculated at 10 mA cm −2 by subtracting the experimental RHE potentials from thermodynamic potential 1.23 V were found to be 250 mV, 270 mV and 280 mV for sample 1, sample 2 and pure Co 3 O 4. Such calculations reveal that the use of natural products of the milky sap of CP as a surface modier for Co 3 O 4 has great potential to enhance the catalytic features of OER electrocatalysts by lowering the energy barrier for the OER process, which is the essential demand in the current studies, and they can also be used to design new functional materials for energy storage and conversion systems. To further understand the OER kinetics, the Tafel slopes were estimated from the linear region of LSV curves, as shown in Fig. 6b. The Tafel slopes obtained for sample 1, sample 2 and pure Co 3 O 4 are 53 mV dec −1 , 63 mV dec −1 and 66 mV dec −1 respectively. The low Tafel slope for sample 1 indicates the favorable and fast OER kinetics on its surface. Such a slow OER accelerated by the newly prepared Co 3 O 4 material is a major advancement in the eld of catalysis that could be used for practical applications. The Tafel slope of 53 mV dec −1 is the lowest to date for the Co 3 O 4 -based OER electrocatalysts in alkaline media. These results indicate the high potential of natural products for the design of efficient nonprecious catalytic materials. Chronopotentiometry was performed to monitor the durability of sample 1 at constant 10 mA cm −2 (see Fig. 6c). In addition, the milky sap of CP has signicantly enhanced the durability of Co 3 O 4 -based sample 1 for 50 hours. There was no abruption in the potential during the test. This excellent durability of sample could be assigned to the good dispersion of Co 3 O 4 and its fascinating structure. Based on this long-term durability experiment, sample 1 might be used for industrial applications. The stability of Co 3 O 4 -based sample 1 was evaluated by plotting the LSV curves before and aer the durability test (see Fig. 6d). It can be observed that the OER onset potential was not altered even aer the period of 50 hours, which reveals the outstanding stability of Co 3 O 4 -based sample 1. Hence, sample 1 has great potential for use in the production of O 2 compared to the electrocatalysts under alkaline conditions recently reported for OERs. The EIS study was performed to gain a deep insight into the charge transport between the working electrode and the electrolyte, which favors the OER process, as shown in Fig. 6e. The EIS data were tted with an equivalent circuit and the corresponding circuit elements were solution resistance (R s ), charge transfer resistance (R ct ) and constant phase element (CPE) corresponding to double-layer capacitance. The calculated charge transfer resistance values for pure Co 3 O 4, sample 1, and sample 2 were found as 823 ohms, 71 ohms, and 612 ohms respectively. The nanostructured Co 3 O 4 sample prepared with low amounts of the milky sap of CP showed fast charge transport compared to pure Co 3 O 4 and sample 2 of Co 3 O 4 prepared with a large amount of the milky sap of CP, as shown in Fig. 6e. The small semi arc of the Nyquit plot is an indicator of low charge transfer resistance and the measured results agreed well with our previous study. 71 Co 3 O 4 is a semiconducting material and the optical band gap of sample 1 was calculated to be about 2.03 eV, which was lower than that of the pure Co 3 O 4 sample and sample 2, hence the conductance of sample 1 is large, which is in good agreement with the EIS information about the charge transfer resistance experienced by sample 1 of 71 ohms. The combined results of optical band gap and EIS studies suggest that sample 1 exhibited high conductance, therefore it has shown highly favorable electrochemical performance. The performance evaluation of Co 3 O 4 prepared with and without the milky sap of CP is presented graphically in terms of the estimated overpotential at two different current densities of 10 mA cm −2 and 50 mA cm −2 , as shown in Fig. 6f. For better visualization, the overpotential of each material was estimated at two different current densities of 10 mA cm −2 and 50 mA cm −2 , and is shown in Fig. 6f. The bar graph representation indicates that sample 1 exhibits a superior electrocatalytic activity even at a higher current density than that of pure Co 3 O 4 , and sample 2. To understand the reason for improved electrocatalytic activity of pure Co 3 O 4 , sample 1 and sample 2, we studied the electrochemically active surface area (ECSA) using CV curves in the non-redox region at different scan rates, as shown in Fig. 7a-c. There is a linear relationship between ECSA and the doublelayer capacitance (C dl ), hence we obtained the CV curves in the potential range of 0.05 to 0.25 versus Ag/AgCl (V) at different scan rates, as shown in Fig. 7a-c. The measured C dl information of pure Co 3 O 4, sample 1, and sample 2 was estimated to be about 1.03 × 10 −2 mF cm −2 , 8.56 × 10 −2 mF cm −2 , and 6.86 × 10 −2 mF cm −2 respectively, as shown in Fig. 7d. Sample 1 exhibited the highest value of ECSA, conrming the easy accessibility of active sites for the electrolyte, which clearly played an important role towards the enhanced OER. Furthermore, the OER performance was evaluated, and the recently published results of the OER are given in Table 2. [78][79][80][81][82][83][84][85][86][87][88][89][90][91][92][93][94][95][96][97] It is obvious that the presented approach is facile, low cost, and efficient in terms of low overpotential, environmental friendliness and scale up for the fabrication of electrocatalyst materials.

Capacitance analysis of milky sap of CP-mediated sCo 3 O 4 nanostructures
The capacitive activity of Co 3 O 4 nanostructures prepared with the milky sap of CP was evaluated by CV using a three-electrode cell set up in 3.0 M KOH electrolyte. For comparison, pure  shown a slight shi in the oxidation potential to a higher value, while the reduction potential towards a lower value with the increase in scan rate, as shown in Fig. 8a,b. This shi in oxidation and reduction of CV curves with the increase in sweep scan rates was assigned to the internal resistance and polarization effect. 74 The nonlinear region of the CV curves conrms the redox properties of the milky sap of CP-mediated Co 3 O 4 and pure Co 3 O 4 and their pseudo capacitance properties. The pseudo-capacitance was found to be highly consistent with the increase in scan rate, suggesting an excellent reversibility of electrochemical redox processes. 75 Moreover, the capacitance properties of pure Co 3 O 4 were studied by employing galvanic charge-discharge (GCD) measurements at different current densities of 0.8, 0.85, 089, and 0.94 A g −1 , as shown in Fig. 9a. The Ir drop in GCD curves as shown in Fig. 9a could be connected to the possible compressive stress, which increased the charging/discharging time, resulting in Ir drop. The GCD curves have shown the nonlinear behavior of pure Co 3 O 4 and supported the claims about the pseudo-capacitance properties made on the CV analysis. The specic capacitance C s , energy density and power density were calculated using the following equations: 76,77  Paper RSC Advances Herein, C s is the specic capacitance, I is the current (A), Dt is the discharge time (s), m is the deposited mass of material (mg), and DV is the potential window (V), E d is the energy density, and P d is the power density.
The C s and energy density values of pure Co 3 O 4 were estimated to be around 300 F g −1 at 0.8 A g −1 and 7 W h kg −1 respectively, as shown in Fig. 9b and c. This low value of specic capacitance indicates that there is immediate need to tune the capacitance properties of pure Co 3 O 4 , and hence, we prepared milky sap of CP-mediated Co 3 O 4 with enhanced Cs and energy density, as shown in Fig. 10. The GCD curves of the milky sap of CP-mediated Co 3 O 4 were measured at different current densities, as shown in Fig. 10a. It is worth noting that the nonlinear behavior is shown with almost a triangular shape and is fully supported by the CV redox behavior, which reveals an excellent pseudo capacitance behavior of milky sap of CP-mediated Co 3 O 4 . The specic capacitance retention percentage of 105% was observed for 900 cycles, which conrmed the excellent cycling stability of the material, whereas Cs of 699 F g −1 at 0.8 A g −1 was observed for milky sap of CP-mediated Co 3 O 4 , as shown in Fig. 10b and c. The retention rate of capacitance increased, as shown in Fig. 10b, aer 900 GCD cycles due to the enhanced electron transport and high specic surface area exhibited by milky sap of CP-mediated Co 3 O 4. This led to the generation of more charge transfer channels in the modied electrode, thereby accelerating the swi ion/electron transfer rate, which further improved the electrochemical activity of milky sap of CP-mediated Co 3 O 4 and stabilized the working electrode.
A coulombic efficiency of more than 80% and an energy density of 30 W h kg −1 were estimated for milky sap of CPmediated Co 3 O 4 , as shown in Fig. 10d and e. This signicant progress in the enhanced capacitance properties of milky sap of CP-mediated Co 3 O 4 could be attributed to the surface modication of nanostructures during the growth process in the presence of capping agents, reducing agents and stabilizing agents derived from the milky sap of CP. The enhanced electrochemical properties of milky sap of CP-mediated Co 3 O 4 (sample 1) could be connected to the surface oxygen vacancies, low charge transfer resistance, low optical band gap, surface modication, and high ECSA values. The presence of capping agents, reducing agents and stabilizing agents together brought the surface modication and surface oxygen vacancies and enabled the high compatibility of milky sap of CP-mediated Co 3 O 4 (sample 1), hence an enhanced electrochemical performance was demonstrated. The estimated values of specic capacitance, energy density, power density, coulombic efficiency, and specic capacitance retention percentages are given in Table 3 for the fast view of presented results. Moreover, we compared the presented capacitance results of milky sap of CPmediated Co 3 O 4 (sample 1) with many of the recent works, as given in Table 4, 98-102 and hereby it is safe to say that the proposed material is better than or equal to many of the recently published supercapacitors in terms of specic capacitance and energy density. It has been shown that the working potential of Co 3 O 4 was in the range of 0 to 0.45 V in alkaline media and the material exhibited pseudo capacitance features described by the CV curves shown in Fig. 8a and b. The mechanism of energy storage is shown in Scheme 3, which illustrates the typical charging-discharging behavior of the electro active material. 98,99 The reversibility of valence state variation of Co 3+ /Co 4+ conrms the quick redox properties of Co 3 O 4 (sample 1). Additionally, the electrochemical redox potential of Co 3+ /Co 4+ transition is shown to be almost the same, therefore the redox peaks are found to be closely overlapping. 100,101

Conclusions
In this study, we used the milky sap of CP to tune the surface properties of Co 3 O 4 nanostructures by a low-temperature aqueous chemical growth method. Physical structure analysis showed a successful reduction in the optical band gap and shape of Co 3 O 4 nanostructures by various reducing, capping and stabilizing agents. The newly prepared Co 3 O 4 nanostructures proved to be highly active electrode materials for OERs and supercapacitor systems. We found the driving role of phytochemicals from the milky sap of CP in enhancing the electrochemical properties of Co 3 O 4 nanostructures. The OER activity was supported by a low overpotential of 250 mV at 10 mA cm −2 and a long durability of 45 hours. The capacitance of Co 3 O 4 nanostructures prepared with low amounts of the milky sap of CP was about 700 F g −1 at 0.8 A g −1 and the specic capacitance retention percentage was found to be about 105% aer 900 GCD continuous cycles, revealing an excellent cycling stability of the material. The reducing, capping, and stabilizing agents from the milky sap of CP improved the morphology, particle size, and surface oxygen vacancies. The obtained results indicated that the synthesis of nanostructured materials using the milky sap of CP could be an effective method to fabricate high-performance electrocatalytic materials for the development of advanced electrochemical devices.

Author contributions
Adeel Liaquat Bhatti, did the material synthesis and partial electrochemical tests. Aneela Tahira, did XRD analysis. Shushel Kumar, FTIR measurement. Zaheer Ahmed Ujjan, did supercapacitor tests. Muhammad Ali Bhatti, did the ECSA and optical band gap s measurements. Sooraj Kumar, did XRD measurement. Umair Aab, did EIS analysis. Amal Karsy, did SEM measurement. Ayman Nafady, did preview of the results and validate them. Antonia Infantes-Molina, did XPS analysis. Zafar Hussain Ibupoto, did the supervision and wrote the original dra of manuscript.

Conflicts of interest
Authors declare no competing interests in the resented research work.